### SlideShare for iOS

by Linkedin Corporation

FREE - On the App Store

From a structural point of view, corrugated board would fit on the category of sandwich structures, which in sectors as aeronautics or construction are today commonly analysed using simulation tools ...

From a structural point of view, corrugated board would fit on the category of sandwich structures, which in sectors as aeronautics or construction are today commonly analysed using simulation tools that are based on the Finite Element Method. However, in spite of similarities to applications in other materials, FEM simulation of corrugated board is a high challenging modelling task due not only to the need of addressing properly the complex mechanical modelling of paper itself, but also because of phenomena that are directly related to the corrugated structure, as the relationships between local and global instability failure modes. The present paper, through a set of application examples, shows how different Abaqus modeling capabilities (SC8R elements, composite sections, connector elements, …) can be applied for solving the different difficulties that arise when modelling corrugated board. The integration of these capabilities has led to the development of virtual prototypes for the two most common corrugated board packages: B1 boxes and agricultural trays. From the experience in these box types, and taking advantage from the inherent modelling simplicity of the composite layered models together to the flexibility offered by the available modelling techniques in Abaqus, these virtual prototypes have been extended as a design tool for very different types of corrugated board packages.

- Total Views
- 1,910
- Views on SlideShare
- 1,910
- Embed Views

- Likes
- 0
- Downloads
- 63
- Comments
- 0

No embeds

Uploaded via SlideShare as Adobe PDF

© All Rights Reserved

- 1. Visit the SIMULIA Resource Center for more customer examples. Design of Different Types of Corrugated Board Packages Using Finite Element Tools M. A. Jiménez-Caballero, I. Conde, B. García, E. Liarte Instituto Tecnológico de Aragón C/ María de Luna 7-8, 50007 Zaragoza. SPAIN www.ita.es Email of corresponding author: majimenez@ita.esAbstract: From a structural point of view, corrugated board would fit on the category ofsandwich structures, which in sectors as aeronautics or construction are today commonlyanalysed using simulation tools that are based on the Finite Element Method. However, in spiteof similarities to applications in other materials, FEM simulation of corrugated board is a highchallenging modelling task due not only to the need of addressing properly the complexmechanical modelling of paper itself, but also because of phenomena that are directly related tothe corrugated structure, as the relationships between local and global instability failure modes.The present paper, through a set of application examples, shows how different Abaqus modellingcapabilities (SC8R elements, composite sections, connector elements, …) can be applied forsolving the different difficulties that arise when modelling corrugated board. The integration ofthese capabilities has led to the development of virtual prototypes for the two most commoncorrugated board packages: B1 boxes and agricultural trays. From the experience in these boxtypes, and taking advantage from the inherent modelling simplicity of the composite layeredmodels together to the flexibility offered by the available modelling techniques in Abaqus, thesevirtual prototypes have been extended as a design tool for very different types of corrugated boardpackages.Keywords: Corrugated Board, Packaging, Box Compression,1. IntroductionFE-based simulation has been increasingly used in the last decades as the main structural analysistool in many different industrial sectors and, in combination with other numerical techniques andtools as CFD, has been also the main basis for the more recent concept of “virtual prototypes”replacing manufacturing and testing of physical components. Starting in the past from civilengineering, aeronautics and automotive industry, present applications of finite element simulationextend to any industry sector as electronics, medical equipment, packaging, and more specificallycorrugated board packaging. In general terms, compression strength can be considered as themost important requirement of a package, or at least the one that is common to all package types,as during transport and storage, any box has to support without damage the weight of the rest ofthe supported boxes; thus, initially, corrugated board industry has considered FEM as a possible2009 SIMULIA Customer Conference 1 Visit the SIMULIA Resource Center for more customer examples.
- 2. tool for replacing the traditional application of semi-empirical expressions (Mc Kee et al. 1963)looking for both, improved accuracy in the prediction of box compression strength usingnumerical simulation of the package (Gilchrist et al. 1999, Rahman 1997, Urbanik et al. 2003,Biancolini et al. 2003), and extending the analysis to package types as different as possible.The introduction process of FE in corrugated board industry has been slower than in other sectors,probably because of the very complex mechanical behaviour of both, paper itself and corrugatedboard, leading to models that require very specific material models or advanced FE techniques.However, and in spite of the slow start-up, applications of FEM to corrugated board industry arerapidly growing, somehow taking advantage of previous developments in advanced modelling ofcomposites and composite sandwich structures, with relevant similarities to corrugated board. Thepresent paper summarises the general aspects of the simulation methodology that the authors areapplying for the structural analysis and design of corrugated board packages. The objective of thepaper is to provide a general description of the practical capabilities of the developed simulationmethodology, showing how Abaqus can be applied in the development process of corrugatedboard packages, but without entering into detailed descriptions of a given finite element model orsimulation, nor presenting geometry and paper composition details of analysed packages.2. GENERAL METHODOLOGY FOR FINITE ELEMENT SIMULATION OF CORRUGATED BOARD2.1 Modelling the mechanical behaviour of paperResulting from the manufacturing process, paper is an orthotropic material with very differentmechanical properties in each of the three principal material orientation directions (Baum et al.1981): through thickness direction (ZD), in-plane direction parallel to rolling during processing,referred as machine direction (MD), and the in-plane direction normal to MD, referred as crossdirection (CD). Apart from orthotropy, paper behaviour exhibits two additional characteristicsthat prevent from application of simple materials models: a) highly non linear behaviour, b) largedifferences between tensile and compressive responses in any of both, MD and CD. Figure 1shows the characteristic shape of the stress-strain curves in MD and CD. stress Tensile curve in MD Tensile curve in CD Compressive curve in CD strain Compressive curve in MD Figure 1. Characteristic stress-strain curves of paper in machine direction (MD) and cross direction (CD).2 2009 SIMULIA Customer Conference
- 3. Of course, paper behaviour exhibits additional characteristics that increase additionally the level ofcomplexity of modelling, as exhibiting significant creep, humidity dependence of mechanicalproperties, higroexpansion, … In any case, it is important to remark that orthotropy, non-linearityand differences tension-compression play all an important role even in the simple case of BCTtesting of a package under controlled room conditions, and because of this, mechanical modellingof paper, even for the simpler loading cases always rely on the availability of a user developedmaterial model implementing as many as possible from the three referred characteristics plusspecific features for handling other property dependences if required by specific application (Xiaet al. 2002, Isaksson et al. 2004, Mäkela et al. 2003, Alfthan et al. 2005). In the examples that arenext presented, an in-plane orthotropic damage model with different treatment of tension andcompression and including definition of final paper failure according to the Tsai-Wu criterion(Tryding, 1994) has been applied for modelling the static response of paper in the short-term usingshell elements; the model has been implement through UMAT and VUMAT user subroutines,only shell element versions, in Abaqus/Standard and Abaqus/Explicit, while the requiredtransverse shear stiffness values for the shells are calculated using the out-of-plane shear elasticmoduli from the constituent papers. The model has been validated at paper level throughvalidation from ECT (edge crush test) and FCT (flat crust test) experimental results (Jiménez et al.2003, Bielsa et al. 2006).Figure 2 summarises as example the validation of the paper material model by simulating inAbaqus/Explicit a FCT test of a single flute board by means of a single wave model in whichsymmetry boundary conditions are applied in all the edges given the large dimensions of the FCTsample (100 mm x 25 mm) when compared to the single wave. Results show how threeexperimental load peaks can be identified along the test with deviations around to 10%. Asalready expected when designing these validation tests, the differences in displacement predictionare higher because of different reasons, including among these the simplifications in the modellingof the adhesive and of the out-of-plane behaviour of the paper 1600 Symmetry conditions for modelling a 100mmx25mm FCT sample 1400C3D8R elements for FCT testadhesive Simulation result 1200 Total failure extension 1000 Load (N) 800 Failure progression 600 Failure initiation at creases 400 200 C3D8R elements S4R elements for liners 0 for adhesive 0 0,5 1 1,5 2 2,5 and fluting Displacement (mm)Figure 2. Comparison of simulation and experimental results for FCT simulation of single flute paperboard.2009 SIMULIA Customer Conference 3
- 4. As it will be presented in forthcoming parts of the paper, carrying trays for agricultural productspresent, in addition to BCT qualification, another key requirement in terms of the so called“bottom sag” under sustained load or creep. This requirement is established in terms ofdisplacement instead of strength, as the limit structural condition is determined by the possibilityof the bottom of a given try touching and damaging the fruits or vegetables that are packaged inthe box underneath. In order to cover creep, the material model of paper has been modified forconsidering viscoelastic strains under sustained loads. The selected model is based on Coffinequation for paper creep (Coffin, 2005) that considers potential and logarithmic behaviour (seeequation 1) and fulfils the needed conditions leading to the possibility of creating master curvesfor paper through a logarithmic time shift in stress values (Brezinski, 1956). Coffin equation forthe creep modulus, J, is shown in Equation 1. J (t ) 1 0 E 1 A 1 e at B ln bt 1 1The first term represents primary creep, which is considered a delayed response where A is theinverse of elastic modulus of the delayed response, a is a time scale factor and is the exponent ofthe potential behaviour observed for short times. The second term represents secondary creep andis based on Brezinski´s observation that long term creep is a lineal function of logarithm of time. Bis a creep flow parameter and b is a time scale factor. Figure 3 shows results from simulation ofpatch tests with a single shell for tensile creep at different percentage of tensile failure stress,together to results of the experimental creep tests that were used for determining the parameters ofthe corresponding creep equation; results correspond to a recycled paper to be used as linerboard. 2.50E-10 2.00E-10 J (1/Pa) 1.50E-10 1.00E-10 — 10% — 20% — 40% 5.00E-11 — Simulation 0.00E+00 0 50000 100000 150000 200000 250000 300000 350000 Tiem po (s) Figure 3. Results of creep characterisation of a sample paper and validation of user creep model for paper through tensile patch testThe modelling methodology that is proposed by the authors for BCT simulations and analysis ofbox bottom sag (including creep) is based on Abaqus/Standard simulations, mainly because ofhigher computational efficiency for most of the analysed cases. In any case, during the initialstages of the methodology development, Abaqus/Explicit was also used from to time to time forvery specific simulations, as an easier way to extend analysis beyond specific instabilities as thosein the FCT example that has been previously presented (Figure 2).4 2009 SIMULIA Customer Conference
- 5. 2.2 Simplified laminated composite modelsModelling of the corrugated structure using 3D shells for liners and fluting, as in the exampleshown in Figure 4, is not realistic when thinking of virtual prototyping for efficient materialselection or analysis of geometry variations. Efficiency problems of 3D shell-based modelling ofcorrugated shape are not only related to computation times for the whole package but also tomodelling details of complex package areas as corners and flaps; in addition, it must be noticedthat strength analysis of paperboard requires non-linear FEM analysis due to the importance ofinstabilities, so requiring some computational effort. Thus, detailed FEM models of corrugatedboard structures, like the ones that are shown in Figure 4, are useful for estimating somecorrugated board properties that are difficult to be measured experimentally, but are not yetrealistic for the modelling and simulation of the whole package when thinking of a large variety ofpackage types. It is important to remark here that simulation difficulties are not only related tocomputational effort but also to the complexity of geometrical modelling. Single fluted board Doubled fluted board 2 3 1 Figure 4. Pictures of single flute and double flute corrugated board and corresponding 3D-shells models with detailed flute geometryFor modelling purposes, corrugated board can be simplified to a laminated structure withalternative “thin” layers of non-corrugated liners, and “thick” layer consisting of a corrugatedpaper flute. Hence, corrugated board is defined structurally as a sandwich structure with anon-continuous core, like other well-known sandwich structures as composite sandwich panelswith honeycomb cores. Thus, a first step for simulation is translating the actual corrugated coregeometry to a set of equivalent mechanical properties to be associated to a continuum core,therefore allowing simulation through any of the different techniques that are used for sandwichstructures (with technique selection depending mainly on sandwich thickness): layered solids,layered thick shells, layered continuum shells, or combinations of previous approaches. Severalmethods can be found in literature for minimising the errors in the in-plane and flexuralbehaviours that are related to the simplifications for establishing the equivalent flue properties(Luo et al. 1992), as well as for estimating transverse shear equivalent properties (Nordstrand et al.1997) for the equivalent structure. In the examples in this paper, estimation of transverse shearstiffness is performed from simulations of detailed corrugated geometry models as in Figure 4, asmodelling of a flat panel for determination of equivalent properties is easy to be parameterised andautomated, even if not suitable for the modelling of the final package.2009 SIMULIA Customer Conference 5
- 6. Once an equivalent material for a continuous core is considered, the most cost-effective elementtype for corrugated board is usually a S4R thick-shell with proper accounting for transverse shearstiffness. Of course, other approaches exist for modelling corrugated board, as using solidelements for the core or using layered solid elements (C38R for instance) instead of layered shells,but some modelling issues, as keeping suitable aspect ratios in the solid elements or reaching tothe required number of through thickness solids for proper accounting of transverse shear, requireusually quite large computational models. However, as it is later presented when discussingbottom sag, such approaches are sometimes required to improve modelling results.Next, Figure 5 shows an example of the CD stresses in a liner for a non-linear buckling analysis ofa corrugated board panel. Results on the left correspond to a detailed FE model with modelling offlute geometry using S4R elements, while results on the right have been obtained from asimplified composite shell model, using a single layer of S4R with a *COMPOSITE sectiondefinition, using equivalent core properties. It is required to remark that detailed modelling of thecorrugated medium implies some restriction for the mesh size in the liners, so in the example ofFigure 5 it is also interesting to note the much coarser mesh size while maintaining the significantstress values (compressive ones) below a 6% difference with regard to the detailed model, whichis a quite low value considering non-linear buckling analysis.Figure 5. Comparison of CD stresses between detailed model including corrugated flute geometry and equivalent composite model.In spite of its simplicity, the application of simplified composite models gives rise to an addedproblem when thinking of failure prediction: a detailed model with flute geometry, as the one inthe left part of Figure 5, could be directly applied for prediction of local instabilities in the casethat the mesh size is properly selected (see Figure 6), but analysis of local bucking in a simplifiedmodel without considering corrugation shape is not so simple.6 2009 SIMULIA Customer Conference
- 7. Figure 6. Detailed FE model for local buckling prediction.As already mentioned, the Tsai-Wu failure criterion is possibly the most usual for paper strengthanalysis. Nevertheless, when paper is used as part of corrugated paperboard, the failure criterionhas to take into account also local buckling as a possible failure mode for the liners, at loadssignificantly lower than those for strength failure. The alternative way for considering localbuckling in simplified models that is followed by the authors consists of combining the Tsai-Wustrength criterion with an additional criterion related to local instability. This approach requiresfor each different corrugated board specific determination of such instability criterion either byanalytical or numerical tools (Nyamn et al 1999, Biancolini et al. 2003), as this depends on thespecific geometry of the supporting corrugation wave. The development and validation of theproposed simulation methodology has been supported by a large experimental program, not onlyat package level, but also in previous development stages through in-plane compression tests ofrectangular corrugated boards using lateral supports for preventing global buckling at low loads.2.3 Selection of element typeAs already mentioned, equivalent composite models are not limited to layered shells but caninclude combinations of different elements, as for instance, shells for liners with solids for thecore, or even layered solid without shells. Like in any FE simulation, the selection of the rightelement is critical. As an example of the relevance of element selection, a numerical andexperimental study for the selection of the most adequate element type for modelling bending incorrugated board panels was carried by the authors (Jiménez et al. 2004). Bottom sag analysis ofbox bottom requires simulation of bending, and therefore, transverse shear stiffness may play animportant role. Not all the element types that can be used for modelling an equivalent laminateconsider transverse shear behaviour with the same accuracy, neither all of them are able to takeinto account possible thinning of corrugated board. The results of the study indicated that a verysimple model of composite linear thick shells with reduced integration (S4R) using simplifiedcontinuum-equivalent properties for the fluting is the most efficient solution for single flutecorrugated board; however, when double fluted boards are of interest, as it is usually the case incarrying trays, importance of shear transverse stiffness and thinning of paperboard increasesignificantly, being highly recommended the using of at least four layers of composite reducedintegration continuum shells (SC8R). Figure 7, from the referred study, illustrates the differencebetween a single flute board and a double flute one. The first graph shows how the compositeshells capture corrugated board stiffness very accurately in a single flute board, the second one2009 SIMULIA Customer Conference 7
- 8. shows how the same elements behaves too stiff when a double flute is analysed, finally, the thirdone shows how using four layers of composite continuum shells (SC8R) solves the problem.Figure 7. Comparison of flexural stiffness prediction capabilities for different types of equivalent composite models.3. Application to papers selection in B1 boxes and agricultural trays3.1 Simulation of BCT testThe BCT (box compression test) value is the most usual property for qualifying packageperformance in corrugated board packages. It consists of the maximum achieved load level underquasi-static compression of the package between two rigid plates in a universal testing machineunder controlled temperature and humidity room conditions. Regarding package functionality, theBCT value refers to the package capability to withstand the weight of the rest of the stack over it.Figure 8 shows an image of a finite element model for simulating the BCT test of a B1-type box,also referred as american box; it includes the final damaged areas together to a picture of a testedsample, showing very good correlation in terms of predicting failure mode. Figure 8. Comparison of BCT simulation with experiment.8 2009 SIMULIA Customer Conference
- 9. The finite element model for the simulation in Figure 8 consists of S4R elements with layeredcomposite definition for the corresponding *SHELL SECTION and definition of connectorelements (type=CONN3D2) for the corner lines. The section behaviour of these connector hasbeen defined after experimental characterisation of the torque/angle behaviour of the folded linesfor the corresponding boards, following recommendations from studies on other paperboardpackages (Beldie et al. 2001). JOIN and REVOLUTE behaviours in the connector sectiondefinition, in combination with the NONLINEAR option in *CONNECTOR ELASTICITY, areapplied when it is required to define non-linear behaviour.For the examples presented in the paper, connector elements are always selected instead of othermeans to accomplish the connection as multipoint constraints. Model sizes are not too big andtherefore the higher efficiency of multi-point constraints is not a key factor, while connectorelements combine very high versatility in connection behaviour with easy definition and theyallow very easy modification of connector type and behaviour details during the initial stages ofmodel development and validation.The larger complexity of the BCT model for a B1 box is the definition of the contacts betweenbox flaps and between these and compression plates (Figure 9 shows an example of a magnifiedglobal buckling behaviour of the top part of a box, with some flaps removed for displayingpurposes). Analysis involves combination of local material failure with global instability,therefore non-linear geometric analysis is required. Because of the relevance of the globalbuckling behaviour when analysing BCT, it is important to account for geometric imperfections ofthe box; in the examples in this paper, this was accomplished by using the option*IMPERFECTION with mode shapes from a previous eigenvalue buckling modes estimationusing *BUCKLE. Figure 9. Finite element model of B1 box (two of the top flaps are removed for displaying purposes) with magnified deformation to show global buckling.2009 SIMULIA Customer Conference 9
- 10. While it is usual that B1 boxes allow symmetry modelling in height (as the model in Figure 9,only for the top half of the box), carrying trays as AGRIPLAT and PLAFORM types foragricultural products allow one-quarter symmetry models (see Figure 10). However, modelling ofthe corner areas adds certain complexity to the modelling tasks, requiring also to keep goodcontrol of material orientation definitions. Modelling of glue lines in corner areas and flaps can bealso carried out by using connector elements. AGRIPLAT type box CD material dir. MD material dir. Detail of material orientation One-quarter PLAFORM type box symmetry FE models Figure 10. FE models of carrying trays for agricultural products, including a example material orientation definition detailsFigure 11 illustrates how the FE simulation of a PLAFORM type carrying try is used for analysingwhich is the effect in BCT value and failure mode of using two possible considerations forincluding a carrying hole in the try lateral side, the first option considers such hole as additional tothe venting hole in the bottom line, while the second one just enlarges the venting hole to therequired size for placing easily the hand. Figure 11 illustrates also how the simulations have beenvalidated experimentally, not only in terms of BCT load value, but also in terms of damaged areasand failure mode.10 2009 SIMULIA Customer Conference
- 11. Double hole: venting and carrying Single larger hole with double function Figure 11. Validation of prediction of global failure areas in PLAFORM type box with different geometry for venting and carrying holesSimulations following the proposed methodology present an error with regard to experimentalBCT values that is usually below 10% in terms of maximum load, which can be considered a verylow error if the complexity of material behaviour and failure mode (combining local buckling andstrength failure) is put together to other simulation details as torque-angle behavior of folded lines,definition of glue lines, or non-linear analysis involving global buckling. Validation of all modeldetails for different packages has required a large experimental effort with monitoring of manydifferent variables during the test, as out-of-plane displacement of package faces or application ofhigh speed cameras for identifying onset of local buckling. Figure 12 shows an example of theexperimental set-up during the initial testing program for model development of agricultural trays. BCT plate LVDTs Acquisition system for LVDTs Acquisition system for LVDTs Data cable from universal test rig Computer Lighting Camera2009 SIMULIA Customer Conference 11
- 12. Figure 12. Experimental set-up for detailed BCT analysis to provide data for FE model development and validation3.2 Simulation of bottom sag in agricultural trays The bottom sag of agriculture carrying trays can be studied with the presentedcomposite models since they reproduce flexural rigidity of corrugated board accurately inthe loading range of interest (Jiménez et al. 2004). The strength requirements from BCTare increased now with stiffness ones; the objective in the design is to avoid excessivedisplacements that would cause the tray bottom to contact with the products in the boxbelow (what happens at load levels well below ultimate bottom sag strength), so requiringconsideration of creep displacements after initial load application. In the example corresponding to the simulation in Figure 13, the tests were performedon a PLAFORM carrying try, measuring the displacement in the centre of the bottom.The load was applied by means of bags filled with of golf balls so that load is distributedin the box bottom. Simulation consisted of one unique step using the procedure*STATIC and specifying the real duration of the test. Load application in time wascontrolled by means of an *AMPLITUDE procedure. The material model included theCoffin model for paper creep already commented in previous points of this paper.Comparison of simulation results to experimental ones for the creep displacement showsa good approximation to prediction of creep displacements. Although it exists adifference in the total predicted displacement value, this is related to the large initialcompliance showed during the experimental process of loading application, because ofthe trays not being perfectly flat, and so with uneven support along test rig. 8 (m) 7 6 Displacement (mm) Desplazamiento(mm) S4R elements 5 4 3 3 2 1 SC8R elements 2 Test 1 1 Ensayo 1 Test 2 2 Ensayo Simulation Simulacion 0 0 2000 4000 6000 8000 10000 Time (min) Tiempo (min) Figure 13. Simulation of bottom sag in agricultural creep and comparison to experimental results in terms of displacement increase in time12 2009 SIMULIA Customer Conference
- 13. 4. Examples of application to other package designsFEM simulation of corrugated board is not limited to B1 boxes or agricultural tries. Usingsimplified-composite linear 3D shells is usually sufficient for most types of analysis, and becauseof this, modelling of almost any package becomes a relatively straight task. Figure 14 showssimulation and test results corresponding to a corrugated ring that is used as reinforcement in thepackaging of washing powder. FE results show a very good prediction of the failure mode. Contact with upper plate for BCT test Unconnected Unconnected nodes for nodes for modelling of modelling of stepped cuts stepped cuts Modeling of gluing lines with MPCs Contact with lower plate for BCT testFigure 14. Simulation of BCT of corrugated inner ring for reinforcement of washing powder packaging Evolution of markets and packaging personalisation generates continuously newpackage types, for which corrugated board remains as a cost-effective andenvironmentally friendly solution. One of the new corrugated board package types ofhighest commercial interest is the ready-to-sell one. Using of stepped cut along box facesfacilitates removal of the top half of the package; therefore, the same package can be usedfirst for transport and later for showing the product in the store shelves, just using quickremoval of top part of the package without the need of taking out one by one the productsinside. Figure 15 shows how an Abaqus models that has developed for analysing how thepresence of stepped cuts modifies failure mode in comparison to the uncut package.Modelling of the stepped cuts is carried out using unconnected nodes in combination toconnector elements for taking into account contact along cut line. The model has beenapplied for analysing the influence of different designs of the stepped-cuts in the finalBCT performance, as the objective is to keep this in the highest possible value whileassuring easy opening of the box without tearing outside provided cut lines.2009 SIMULIA Customer Conference 13
- 14. Simulation of stepped die-cuts Conecto rigidez by means of connector elements along unconnected node lines Figure 15. FE model of ready-to-sell box for analysis influence of stepped-cuts design on BCT performance5. Conclusions Because of their broad range of simulation procedures and element types, together tothe large possibilities offered by user subroutines, Abaqus provides the requiredframework for the development of a virtual prototyping framework for the corrugatedboard industry. Presented results show that Abaqus application offers possibilitiesranging from selection of constituent papers or flute geometry, to detailed design ofpackage geometry for a set of given performance requirements. Although it has not been referred in the present paper, FEM in general, andparticularly Abaqus thanks to its advanced features, offers to the paperboard industryother possible applications as analysis of board manipulation processes for packageproduction, or even prediction of macroscopic paper performance from microstructuredetails resulting from manufacturing process.6. References1. J. Alfthan, P. Gudmundson. “Linear constitutive model for mechano-sorptive creep in paper”. International Journal of Solids and Structures, 42, 2005.2. L. Beldie; G. Sandberg; L. Sandberg, “Paperboard packages exposed to static loads-finite element modelling and experiments“ Packaging technology & science, vol. 14, 2001.3. Brezinski, J. P. “The creep properties of paper”. Tappi Journal 39(2), 1956.4. G.A. Baum, D.C., Brennan and CC .Habeger, Orthotropic elastic constants of paper, Tappi Journal, Vol. 64, 1981.14 2009 SIMULIA Customer Conference
- 15. 5. M. E. Biancolini and C. Brutti, “Numerical and experimental investigation of the strength of corrugated board packages”, Packaging Technology and Science, Vol. 16(2), March 2003.6. J.M. Bielsa, R. Rodriguez, L. Vila, M. A. Jiménez, “Parametrized finite element analysis of tribological instabilities on polymer-metal sliding contacts”, III ECCM, Lisbon 2006.7. Coffin, D. W., “The creep response of paper”, 13th Fundamental Research Symposium, Cambridge, 20058. A.C. Gilchrist, J.C. Suhling, T.J. Urbanik. “Nonlinear finite element modeling of corrugated board”. Mechanics of Cellulosic Materials, 1999, AMD-Vol. 231/MD-Vol. 85, 1999.9. P. Isaksson, R. Hägglundb,P. Gradina. “Continuum damage mechanics applied to paper”. International Journal of Solids and Structures, 41, 2004.10. M.A. Jiménez, I. Conde, E. Liarte, E. Mozas. “Modelling of bending in a corrugated board”, International Paper Physics Seminar, Trondheim 200411. M.A. Jiménez, E. Liarte. “Simulation of the Edge Crush Test of corrugated paperboard using Abaqus”, Abaqus World Users Conference 2003, Munich.12. P. Mäkelä, S. Östlund. “Orthotropic elastic–plastic material model for paper materials”. International Journal of Solids and Structures, 40, 2003.13. R.C. Mc Kee, J.W. Gander, J.R. Wachuta. “Compression Strength Formula for Corrugated Board”. Paperboard Packaging, Aug 196314. T. Nordstrand, L.A. Carlsson, Evaluation of Transverse Shear Stiffness of Structural Core Sandwich Plates, Composite Structures, Vol. 37, 1997.15. U. Nyman, P.J. Gustafsson, “Local buckling of corrugated board facings, Proceedings of the European Conference on Computational Mechanics”, Munich 1999.16. S. Luo, J. C. Suhling, The bending stiffness of corrugated board, Mechanics of Cellulosic Materials AMD-Vol. 145/MD-Vol. 36, 1992.17. A.A. Rahman. “Finite Element Buckling Analysis of Corrugated Fiberboard Panels”. ASME Symposium on Cellulosic Materials, AMD-Vol.221, 1997, Evanston.18. J. Tryding, A modification of the Tsai-Wu failure criterion for the biaxial strength of paper, Tappi Journal, Vol. 77, 199419. T.J. Urbanik, E.P. Saliklis. “Finite element corroboration of buckling phenomena observed in corrugated boxes”. Wood and Fiber Science, 35(3), 2003.20. Q.S. Xia, M.C. Boyce, D.M. Parks. “A Constitutive Model for the Anisotropic Elastic-Plastic Deformation of Paper and Paperboard”. Int. Journal of Solids and Structures, 39, 2002.7. AcknowledgmentsThis paper presents results from a research programme carried out with the support from SAICA.The authors thank specially to the personnel of the Research and Development Laboratory ofSAICA for their invaluable contributions in the preparation and experimental characterisation ofpaper, corrugated board and packages, as well as in all the practical aspects related to corrugatedboard processing and package converting.2009 SIMULIA Customer Conference 15 Visit the SIMULIA Resource Center for more customer examples.

Full NameComment goes here.